data_1000051
_cod_database_code               ?
_structure_refined               no
_mpod_phase_name                 Pb(Zn1/3Nb2/3)O3-PbTiO3(0.07)
_chemical_formula_sum            'Pb Nb0.62 Zn0.31 Ti0.07 O3'
_mpod_phase_generic_name         PZN-PT
_mpod_symmetry_point_group_name_h-m 3m
_cell_length_a                   ?
_cell_length_c                   ?
loop_
_publ_author_name
'Zhang R.'
'Jiang B.'
'Jiang W.'
'Cao W.'
_publ_section_title
;Complete set of elastic, dielectric, and piezoelectric coefficients of
 0.93Pb(Zn1/3Nb2/3)O3-0.07PbTiO3 single crystal poled along [011]
;
_journal_name_full               'Applied Physics Letters'
_journal_volume                  89
_journal_issue                   24
_journal_article_reference       242908
_journal_pages_number            3
_journal_year                    2006
_mpod_phase_density              8038.4
_mpod_phase_transition_temperature_rhomb_tetra ?
_mpod_phase_transition_temperature_curie ?
_prop_measurement_poling         '[011]c'
_prop_symmetry_point_group_name_h-m mm2
_prop_frame                      '1=[0-11]c 2=[100]c 3=[011]c'
loop_
_prop_conditions_label
_prop_conditions_frequency
1 10000
2 1
3 ?
loop_
_prop_dielectric_tensorial_index
_prop_dielectric_condition_label
_prop_dielectric_measurement_method
_prop_dielectric_permittivity_relative_epsrijS
_prop_dielectric_permittivity_relative_epsrijT
_prop_dielectric_stiffness_relative_betrijS
_prop_dielectric_stiffness_relative_betrijT
11 2 CAP ? 8240 ? 1.2136
22 2 CAP ? 1865 ? 5.3619
33 2 CAP ? 3180 ? 3.1440
11 1 CAP 6953 ? 1.4383 ?
22 1 CAP 1847 ? 5.4150 ?
33 1 CAP 291 ? 34.3440 ?
loop_
_prop_elastic_tensorial_index
_prop_elastic_condition_label
_prop_elastic_measurement_method
_prop_elastic_compliance_sijD
_prop_elastic_compliance_sijE
_prop_elastic_stiffness_cijD
_prop_elastic_stiffness_cijE
11 3 RUS 59.4003 67.5153 173.987 145
12 3 RUS -35.3773 -60.1637 211.639 153.16
13 3 RUS -16.1684 3.3551 114.275 126.66
22 3 RUS 26.2949 102.0024 180.240 180.24
23 3 RUS 5.1644 -54.4683 125.014 150
33 3 RUS 15.0523 62.0233 146.292 141
44 3 RUS 15.2998 15.4512 65.360 64.72
55 3 RUS 245.9933 291.5452 40.65 34.3
66 3 RUS 14.0845 14.0845 71.000 71
loop_
_prop_electromechanical_coupling_tensorial_index
_prop_electromechanical_coupling_condition_label
_prop_electromechanical_coupling_measurement_method
_prop_electromechanical_coupling_kij
15 3 RUS 0.4
24 3 RUS 0.1
31 3 RUS 0.35
32 3 RUS 0.86
33 3 RUS 0.87
loop_
_prop_piezoelectric_tensorial_index
_prop_piezoelectric_condition_label
_prop_piezoelectric_measurement_method
_prop_piezoelectric_dij
_prop_piezoelectric_eij
_prop_piezoelectric_gij
_prop_piezoelectric_hij
15 3 RUS 1823 6.2529 2.49873 1.0158
24 3 RUS 50 3.2360 0.30280 1.9791
31 3 RUS 478 -8.6446 1.69770 -33.5315
32 3 RUS -1460 -17.4399 -5.18545 -67.6476
33 3 RUS 1150 3.6935 4.08443 14.3266
